| ||Format||Pages||Price|| |
|13||$51.00||  ADD TO CART|
|Hardcopy (shipping and handling)||13||$51.00||  ADD TO CART|
|Standard + Redline PDF Bundle||26||$61.20||  ADD TO CART|
This specification covers alloy steel and stainless steel bolting material for pressure vessels, valves, flanges, and fittings for high temperature or high pressure service, or other special purpose applications. Ferritic steels shall be properly heat treated as best suits the high temperature characteristics of each grade. Immediately after rolling or forging, the bolting material shall be allowed to cool to a temperature below the cooling transformation range. The chemical composition requirements for each alloy are presented in details. The steel shall not contain an unspecified element for ordered grade to the extent that the steel conforms to the requirements of another grade for which that element is a specified element. The tensile property and hardness property requirements are discussed, the tensile property requirement is highlighted by a full size fasteners, wedge tensile testing.
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
1.1 This specification covers alloy and stainless steel bolting materials and bolting components for pressure vessels, valves, flanges, and fittings for high temperature or high pressure service, or other special purpose applications. See Specification for the definition of bolting. Bars and wire shall be hot-wrought and may be further processed by centerless grinding or by cold drawing. Austenitic stainless steel may be carbide solution treated or carbide solution treated and strain-hardened. When strain hardened austenitic stainless steel is ordered, the purchaser should take special care to ensure that is thoroughly understood.
1.2 Several grades are covered, including ferritic steels and austenitic stainless steels designated B5, B8, and so forth. Selection will depend upon design, service conditions, mechanical properties, and high temperature characteristics.
1.3 The following referenced general requirements are indispensable for application of this specification: Specification .
Note 1: The committee formulating this specification has included several steel types that have been rather extensively used for the present purpose. Other compositions will be considered for inclusion by the committee from time to time as the need becomes apparent.
Note 2: For grades of alloy-steel bolting suitable for use at the lower range of high temperature applications, reference should be made to Specification .
Note 3: For grades of alloy-steel bolting suitable for use in low temperature applications, reference should be made to Specification .
1.4 Nuts for use with bolting are covered in Section .
1.5 Supplementary Requirements are provided for use at the option of the purchaser. The supplementary requirements shall apply only when specified in the purchase order or contract.
1.6 This specification is expressed in both inch-pound units and in SI units; however, unless the purchase order or contract specifies the applicable M specification designation (SI units), the inch-pound units shall apply.
1.7 The values stated in either SI units or inch-pound units are to be regarded separately as standard. Within the text, the SI units are shown in brackets. The values stated in each system may not be exact equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in non-conformance with the standard.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
A153/A153M Specification for Zinc Coating (Hot-Dip) on Iron and Steel Hardware
A194/A194M Specification for Carbon Steel, Alloy Steel, and Stainless Steel Nuts for Bolts for High Pressure or High Temperature Service, or Both
A320/A320M Specification for Alloy-Steel and Stainless Steel Bolting for Low-Temperature Service
A354 Specification for Quenched and Tempered Alloy Steel Bolts, Studs, and Other Externally Threaded Fasteners
A788/A788M Specification for Steel Forgings, General Requirements
A962/A962M Specification for Common Requirements for Bolting Intended for Use at Any Temperature from Cryogenic to the Creep Range
B633 Specification for Electrodeposited Coatings of Zinc on Iron and Steel
B695 Specification for Coatings of Zinc Mechanically Deposited on Iron and Steel
B696 Specification for Coatings of Cadmium Mechanically Deposited
B766 Specification for Electrodeposited Coatings of Cadmium
E18 Test Methods for Rockwell Hardness of Metallic Materials
E21 Test Methods for Elevated Temperature Tension Tests of Metallic Materials
E112 Test Methods for Determining Average Grain Size
E139 Test Methods for Conducting Creep, Creep-Rupture, and Stress-Rupture Tests of Metallic Materials
E150 Recommended Practice for Conducting Creep and Creep-Rupture Tension Tests of Metallic Materials Under Conditions of Rapid Heating and Short Times
E151 Recommended Practice for Tension Tests of Metallic Materials at Elevated Temperatures with Rapid Heating and Conventional or Rapid Strain Rates
E292 Test Methods for Conducting Time-for-Rupture Notch Tension Tests of Materials
E328 Test Methods for Stress Relaxation for Materials and Structures
E566 Practice for Electromagnetic (Eddy Current) Sorting of Ferrous Metals
E709 Guide for Magnetic Particle Testing
F606 Test Methods for Determining the Mechanical Properties of Externally and Internally Threaded Fasteners, Washers, and Rivets (Metric) F0606_F0606M
F1940 Test Method for Process Control Verification to Prevent Hydrogen Embrittlement in Plated or Coated Fasteners
F1941 Specification for Electrodeposited Coatings on Threaded Fasteners (Metric) F1941_F1941M
F2329 Specification for Zinc Coating, Hot-Dip, Requirements for Application to Carbon and Alloy Steel Bolts, Screws, Washers, Nuts, and Special Threaded Fasteners
ASME StandardsB18.2.1 B220.127.116.11M Metric Heavy Hex Screws B18.3.1M Metric Socket Head Cap Screws B18.3
AIAG StandardAIAG B-5
ICS Number Code 21.060.01 (Fasteners in general); 77.080.20 (Steels)
UNSPSC Code 31161600(Bolts)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM A193 / A193M-16, Standard Specification for Alloy-Steel and Stainless Steel Bolting for High Temperature or High Pressure Service and Other Special Purpose Applications, ASTM International, West Conshohocken, PA, 2016, www.astm.orgBack to Top